Comparison of Shear Bond Strength, Adhesive Remnant Index and Enamel Cracks in Bonding and Rebonding of Stainless Steel Brackets to Enamel Surface Conditioned with Er:YAG Laser Versus Conventional Acid Etching
Objectives: The aim of the present study was to compare shear bond strength (SBS), adhesive remnant index and enamel cracks in bonding and rebonding of brackets to enamel, conditioned with erbium-doped yttrium aluminium garnet (Er:YAG) laser and conventional acid-etching.
Materials and Methods: Fifty-two bovine lower incisors were randomly divided into four groups consisting of group 1 (acid-conditioning in both bondings), group 2 (acid-conditioning in first and laser-conditioning in second bonding), group 3 (laser-conditioning in first- and acid-conditioning in second bonding), and group 4 (laser-conditioning in both bondings). After bracket placement, the samples were thermocycled and tested for SBS in both bonding procedures. Adhesive remnant index scores and enamel cracks were also determined. Tukey's test and one-way analysis of variance was used for statistical analysis (P<0.05).
Results: Mean SBS in the first bonding was 23.59MPa in groups 1 and 2, and 6.9MPa in groups 3 and 4. (P<0.001). The acid-etched teeth had a significantly lower SBS in rebonding, regardless of the reconditioning method (P<0.001). The SBS of the teeth conditioned with Er:YAG laser in the first bonding did not show significant changes in rebonding, although mean SBS was higher compared to the first bonding (P=0.675). Bonding most often failed at the enamel-adhesive interface and enamel cracks were observed in a few teeth.
Conclusion: The method of primary enamel preparation can affect SBS in rebonding. Based on our results, the mean SBS of Er:YAG-conditioned groups was clinically acceptable in bonding and rebonding, although it was lower compared to the acid-etched samples.
2. Newman GV. Epoxy adhesives for orthodontic attachments: progress report. Am J Orthod. 1965 Dec;51(12):901-12.
3. Rosa BT, Perdigão J. Bond strengths of nonrinsing adhesives. Quintessence Int. 2000 May;31(5):353-8.
4. Stern RH, Sognnaes RF. Laser effect on dental hard tissues. A PRELIMINARY REPORT. J South Calif State Dent Assoc. 1965 Jan;33(1):17-9.
5. Han RQ, Yang K, Ji LF, Ling C. Analysis of Shear Bond Strength and Morphology of Er:YAG Laser-Recycled Ceramic Orthodontic Brackets. Biomed Res Int. 2016;2016:7276287.
6. Walsh JT Jr, Cummings JP. Effect of the dynamic optical properties of water on midinfrared laser ablation. Lasers Surg Med. 1994;15(3):295-305.
7. Hosseini MH, Namvar F, Chalipa J, Saber K, Chiniforush N, Sarmadi S, et al. Comparison of Shear Bond Strength of Orthodontic Brackets Bonded to Enamel Prepared By Er:YAG Laser and Conventional Acid-Etching. J Dent (Tehran). 2012 Winter;9(1):20-6.
8. Gokcelik A, Ozel Y, Ozel E, Arhun N, Attar N, Firatli S, et al. The influence of Er:YAG laser conditioning versus self-etching adhesives with acid etching on the shear bond strength of orthodontic brackets. Photomed Laser Surg. 2007 Dec;25(6):508-12.
9. Lee BS, Hsieh TT, Lee YL, Lan WH, Hsu YJ, Wen PH, et al. Bond strengths of orthodontic bracket after acid-etched, Er:YAG laser-irradiated and combined treatment on enamel surface. Angle Orthod. 2003 Oct;73(5):565-70.
10. Martínez-Insua A, Da Silva Dominguez L, Rivera FG, Santana-Penín UA. Differences in bonding to acid-etched or Er:YAG-laser-treated enamel and dentin surfaces. J Prosthet Dent. 2000 Sep;84(3):280-8.
11. Artun J, Bergland S. Clinical trials with crystal growth conditioning as an alternative to acid-etch enamel pretreatment. Am J Orthod. 1984 Apr;85(4):333-40.
12. Kunjappan S, Kumaar V, Prithiviraj, Vasanthan, Khalid SA, Paul J. The effect of bleaching of teeth on the bond strength of brackets: An in vitro study. J Pharm Bioallied Sci. 2013 Jun;5(Suppl 1):S17-20.
13. Loretto SC, Braz R, Lyra AM, Lopes LM. Influence of photopolymerization light source on enamel shear bond strength after bleaching. Braz Dent J. 2004;15(2):133-7.
14. Attrill DC, Farrar SR, King TA, Dickinson MR, Davies RM, Blinkhorn AS. Er: YAG (λ= 2.94 µm) laser etching of dental enamel as an alternative to acid etching. Lasers Med Sci. 2000 Sep;15(3):154-61.
15. Lee BS, Hsieh TT, Lee YL, Lan WH, Hsu YJ, Wen PH, et al. Bond strengths of orthodontic bracket after acid-etched, Er:YAG laser-irradiated and combined treatment on enamel surface. Angle Orthod. 2003 Oct;73(5):565-70.
16. Başaran G, Hamamcı N, Akkurt A. Shear bond strength of bonding to enamel with different laser irradiation distances. Lasers Med Sci. 2011 Mar;26(2):149-56.
17. Walsh LJ, Abood D, Brockhurst PJ. Bonding of resin composite to carbon dioxide laser-modified human enamel. Dent Mater. 1994 May;10(3):162-6.
18. Ozer T, Başaran G, Berk N. Laser etching of enamel for orthodontic bonding. Am J Orthod Dentofacial Orthop. 2008 Aug;134(2):193-7.
19. Türköz C, Ulusoy C. Evaluation of different enamel conditioning techniques for orthodontic bonding. Korean J Orthod. 2012 Feb;42(1):32-8.
20. von Fraunhofer JA, Allen DJ, Orbell GM. Laser etching of enamel for direct bonding. Angle Orthod. 1993 Spring;63(1):73-6.
21. Uşümez S, Orhan M, Uşümez A. Laser etching of enamel for direct bonding with an Er,Cr:YSGG hydrokinetic laser system. Am J Orthod Dentofacial Orthop. 2002 Dec;122(6):649-56.
22. Roberts-Harry DP. Laser etching of teeth for orthodontic bracket placement: a preliminary clinical study. Lasers Surg Med. 1992;12(5):467-70.
23. Oshagh M, Pakshir HR, Najafi HZ, Naseri MM, Nasrabadi NI, Torkan S. Comparison of the shear bond strength of orthodontic brackets in bonding and rebonding: preparation with laser versus conventional acid etch technique. Photomed Laser Surg. 2013 Aug;31(8):360-4.
|Issue||Vol 18 (Continuously Published Article-Based)|
|Lasers Orthodontics Phosphoric Acids Dental Etching|
|Rights and permissions|
|This work is licensed under a Creative Commons Attribution-NonCommercial 4.0 International License.|